Deoxidation of low-alloy steel and saving of ferroalloys
Post on 12-Aug-2016
Embed Size (px)
Iron ore consumption remains almost unchanged and manganese ore consumption amounts to 20 kg/t of steel.
It should be noted, that ferromanganese consumption was 6,8 kg/t of steel in furnace No. 3 and 7.3 kg/t in furnace No. 8, whtle the planned quantity was 7.5 kg/t; some heats were carried out with "their own" man- ganese.
In September, October and November, 1957, the plant was using a new method of charging: 2-3 t of manganese ore before the limestone. The stoppages of furnaces on hearth fettling did not increase and the duration of the heat was reduced by 30-40 rain. On account of the reduction of input of loose materials and deoxidizer, a saving of 144 thousand rubles was made in October and 106 thousand rubies in November.
DEOXIDAT ION OF LOW-ALLO~C STEEL AND SAVING OF FERROALLOYS
Gand. Tech . Sc i . I . M. Le ik in
Central Scientific Research Yalstimte of Ferrous Metalinrgy
As a rule, the majority low-alloy steels are subjected, in the process of manufaeutre, to a preliminary deoxidation of metal in the furnace with silicomanganese or ferromanganese and blast-furnace ferrosiltcon. This method allows not only the deoxidation of steel but also its alloying with manganese.
The quality of steel is better if a complex deoxidizer- silicomanganese- is used. If, however, a strict procedure of adding ferromanganese and blast-furnace ferrosilicon in the preliminary deoxidation is observed, a good quality steel, not inferior to the steel deoxidized in the furnace with silicomanganese, the ratio Mn : Si being(3-4) : 1, can be obtained.
Itence, in the manufacture of low-alloy steels whose carbon content is such that it allows a preliminary deoxidation with ferromanganese and blast-furnace ferrosilicon, the above method may by considered accept- able. It should be noted that silicomanganese, especially with low carbon content, is a scarce ferroalloy.
The ratio of manganese to silicon, and the content of aluminum in the materials charged on the preliminary deoxidation of ferroalloys, have a marked effect on the content of nonmetallic inclusions, most of all oxides, in steel. The increase in the ratio of manganese to silicon and the decrease in aluminum content assist in reducing the amount of oxide inclusibns which remain in steel.
With a view to lowering the consumption of silicomanganese, it is justified in several cases to replace part of it with blast-furnace ferromanganese.
On deoxidation of steels of relatively low carbon content (0.12-0.15%), it is possible to partly repJace silicomanganese by ferromanganese by introducing first ferromanganese and then, after a few minutes, silico- manganese. Immediately after the introduction of ferromanganese, the bath begins to boil vigorously as a remlt of the rapid local increase of carbon concentration. As the experience of the Alchevsk Combine showed, a substantial part of carbon, introduced with ferromauganese, is oxidized before the introduction of silicoman- gananese if the above method of deoxidation is used. It must be taken into account that in this case the total loss of manganese will increase somewhat. The Increase in the loss will depend on the interval between the introduction of ferromanganese and the introduction of silicomanganese.
The consumption of ferromanganese or siIicomanganese in the processing of any steel may be reduced at the expense of increasing the manganese content in steel before the time of deoxidation, and by reducing the loss of manganese during the process of deoxidizing and alloying of steel. The consumption of Fe-Mn and SI-Mn is very effectively reduced if manganese ore is used. Manganese ore (0.75-1.5o7~ should be added after the removal of slag during the formation of secondary slag. A second (smaller) portion of ore may be introduced
at the beginning of the pure boil period, provided that the carbon content and thermal conditions of the process are suitable. A high temperature in the furnace and a small slag layer promote a better utilization of manganese from the ore.
The experience of the open-hearth furnace plant at the Alchevsk Combine, where the scrap-ore process is used shows that when 0.8-1.0~ of manganese ore is added during the period of slag formation, the manganese content in the metal reaches 0.28-0.32% at about 0.1% carbon content.
The high thermal capacity of modern open-hearth furnaces reduces the effect of manganese ore additions oll the frothing of slag to a considerable degree. An increased manganese content in the metal before the de- oxidation makes possible, in addition to the saving of manganese, the application of ferroalloys with a lower ratio Mn : C. This fact is especially important in the manufacture of low-carbon steel with high manganese content.
The loss in burning of manganese and also of chromium (during chromium-containing steel production) depends on the residence time of deoxidants in the furnace. Other conditions being equal, the longer the residence time of ferroalloys in the furnace the higher the loss of deoxidizing elements.
N.N. Dobroldlotov recommends the calculation of the residence time of metal in the furnace by the fol- lowing formula:
z =, l:Sq rain. P
where q is the quantity of ferroalloys introduced, kg; P'is the output of the open-hearth furnace, t /24 hrs.
In the case of steel grade 19G, made in a 250-t furnace when a preliminary deoxidation with ferroman- ganese and blast-furnace ferrosilicon is applied, the residence time is:
1.5.6500 z - - -~17min .
and in case of deoxidation with silicomanganese
1.5.3500 z - ~ 10 rain.
Actually, the duration of preliminary deoxidation for manganese and silicomanganese steels in 180-250 t open-hearth furnaces may constitute 10-15 min and for chromium steels 20-25 rain.
The carbon content in metal before deoxidation affects the loss of manganese. From this point of view, it is preferable to use silicomanganese because in this case the deoxidation can be started at a higher carbon content.
Nowadays, the method of making killed steel without preliminary deoxidation with ferrosilicon in the furnace, i.e. tapping of steel "on the boil"; is becoming widely used. Experience has shown that this method allows a shortening of the heat, a reduction of steel cost and some reduction in the content of phosphorus, hydrogen and nonmetallic inclusions in steel. Tapping of steel without preliminary deoxidation may also be very effective in the case of low-alloy steels, especially steels with low carbon and high manganese content.
According to the information of one of the works, the introduction of all th~ necessary manganese in the form of silicomanganese in combination with the addition of manganese ore in the course of the process, al- lowed a saving of about 20% of silicomanganese in the production of low-carbon silicomanganese steel. In the production of this steel, the preliminary addition into the furnace of 7 kg/t of blast-furnace ferromanganese in combination with the introduction of manganese ore in the course of the steelmaking process and of silico- manganese into the ladle, reduced the consumption of silicomanganese by approximately 35% compared with its consumption in the ordinary method of steel deoxidation.
IJl the production of low-alloy chromium steels with an increased silicon content, it is very appropriate to use any grade silicochromtum by introducing it into the ladle, for alloying steel with chromium and silicon. The melting temperature of silicochromium is considerably lower than the melting temperature of ferrochromium m,d therek)rc the application of silicochromium facilitates the: change over to the manufacture of chromium steel with tapping "on the boi l ' . The alloying of steel with 8i-Cr in the ladle allows a reduction of chromium c(msumptiou on account of a decrease in loss of chromium in burning. The high temperature of steel at the time of tapping attained in modernopen-hearthfurnaees into the ladle, with basic roofs makes it possible to add a larvae quanl:ity of ferroalloy, approaching 20-22 kg/t , as shown by the practice of several works (Alchevsk, Sl:alino),
An improvement in the quality of steel and a saving of ferroalloy may also be achieved by introducing preliminarily me/ted ferroalloys and alloying materials into the ladle. This method necessitates special equipment for melting the additions.
As a rule. low-alloy steels are deoxidized in the ladle with aluminum, and most steels with titanium aim. The amount of aluminum and titanium (ferrotitanium) depends on the grade of steel, its use and the properties rc.quired.
On deoxidation with aluminum, refractory alumina is produced and its inclusions to a great extent remain in the steel. The products of titanium deoxidation have a lower melting temperature and hence the ,mnmetal- lic i.clusions, formed in the process, coagulate more easily and rise to the surface of the metal. Titanium and aluminum lower the tendency of steel to cold shortness and aging, the effect of these elements being bound with their ability to reduce grain size.
It is very important, especially from the point of view of weldability, to take into account the effect of alnlniuum and titanium additions on the lowering of the tendency of steel to grain growth at high temperature. Titanium vigorously combines with the nitrogen present in steel. Finely dispersed particles of titanium com- pomlds forming ill the process of steel solidification, constitute crystallization centers which cause the steel !;rain to become finer. The addition of titanium improves the mechanical characteristics of low-alloy steel, raises the yield point and the ultimate tensile strength. The optimum quantity of titanium addition should be determined for each grade of steel depending on its use and the thickness of plate or section rolled. In prac- tice, in the production of low-alloy steel, the amount of ferrotitanium (25% Ti) introduced as the technological addition constitutes 0.75-2.5 kg/ t of steel. In some low-alloy steels, titanium constitutes one of the alloying ~:lements. Iii this Case the necessary addition of Fe-TI is determined by the required content of titanium in steel.
In the determination of the optimum amount of aluminum addition for a given steel, it is necessary to take into account that the increase in the quantity of aluminum causes the lowering of the fluidity of steel. This, in turn, causes an increase in the contamination of steel with nonmetallic inclusions. The problem of the quantity of aluminmn addition to steel with high manganese and silicon contents should be approached with special caution. According to some data, an increase of aluminum addition to such steel causes an in- crease in the percentage of rejected plates due to seams.
The effect of aluminum on the reduction of grain size and the lowering of the tendency of steel to cold shortness and aging depends to a large degree on the content of metallic aluminum retained in steel, which content depends on the amount of added aluminum and the degree of its utilization. Therefore, it is neces- sary to thoroughly work out the method of introducing aluminum into liquid steel. The aluminum, intro- duced with ferrotitanium (which contains about 7% A1) and ferrosilicon, should also be taken into account.
In the commonly applied method where aluminum is introduced in lumps under the stream of metal in the ladle, the loss of aluminum constitutes 65-85%. The method of adding aluminum into the ladle by means of a rod is a very effective one. The method used in Germany, of adding aluminum to metal aker a pre- determined time in the ladle, may also be mentioned here. In this method aluminum, in iron tubes open at the bottom ends, is immersed in the ladle (see figure). The diameter and the number of robes is chosen in such a way that when the required quantity of aluminum is to be introduced, the height of the tube is equal to the full height of the metal in the ladle. Tests have shown that tubes, filled with aluminum and im- mersed in liquid metal, begin to melt at the lower end.
Method of introducingdeoxidants into metal by means of robes: 1 - liquid metal} 2 - slag; 8 - attachment for introducing the tubes; 4 - tubes with deoxidants.
The dissolution of aluminum takes place gradually as the tubes melt. When this method of introducing aluminum was used, the amount of nonmetallic inclusions in steel proved to be considerably lower and the content of metallic aluminum higher.
NEW EQUIPMENT FOR T I lE EVACUATION OF L IQUID STEEL
Eng. G. A. Soko lov and Pro f . Dr . Techo Sc i . G. N. O iks
Moscow Steel Institute
In the steelmaking plant of the Stalingrad Metallurgical Works "Krasnyi Oktiabr'," new vacuum equip- merit*for the degasification of.liquid steel under vacuum in the ladle, during the transfer of steel from one ladle to another placed in a vacuum chamber, for bottom pouring of steel under vacuum and for top pouring of steel in neutral and protective media, has been erected and put into operation. The weight of treated steel conforms with the charge of electric furnaces, i.e., 12 and 20 t.
The vacuum equipment consists of the following main units: pump station, chamber for the evacuation of steel in the ladle and during the transfer, vacuum chamber for bottom pouring and special molds for top pouring of steel under vacuum.
The chamber for the evacuation of steel in the ladle (Fig. 1). The base of the chamber fs a cylinder of 8300 mm diameter and 2200 mm high, welded from steel plate 12:mm thick. The lid of the chamber is flat, welded and 800 mm high. The body and the lid are reinforced with ribs. Total volume of the chamber is
~ The design of the equipment was carried out at the Works under the supervision and with the direct partici- pation of the co-workers of~he Moscow Steel Institute. Engineers of the Design Department of the Works, V. M. Skvortsov, V. S. Kiriukhin I M. V. Podskrebov, G. I. Kozlitin et al, took part in the design work.